# Ms Theses Ls Dyna

date post

16-Oct-2015Category

## Documents

view

128download

14

Embed Size (px)

### Transcript of Ms Theses Ls Dyna

FINITE ELEMENT SIMULATIONS OF BALLISTIC IMPACT ON METAL AND COMPOSITE PLATES

A Thesis by

Sai Kiran Chelluru

B.E., Andhra University, 2004

Submitted to the Department of Mechanical Engineering and the faculty of the Graduate School of

Wichita State University in partial fulfillment of

Masters of Science

December 2007

Copyrights by [ Sai Kiran Chelluru],

All Rights Reserved

FINITE ELEMENT SIMULATIONS OF BALLISTIC IMPACT ON METAL AND COMPOSITE PLATES

The following faculty members have examined the final copy of this thesis for form and content

and recommend that it be accepted in partial fulfillment of the requirements for the degree of

Master of Science, with a major in Mechanical Engineering

_____________________________________________ Hamid M. Lankarani, Committee Chair

We have read this thesis and recommend its acceptance:

_________________________________________________ Kurt Soschinske, Committee Member

___________________________________________________ Krishna Krishnan, Committee Member

iii

DEDICATION

To My Parents Kameswara Rao and VijayaLakshmi

iv

ACKNOWLEDGEMENTS

I take this opportunity to extend my sincere gratitude and appreciation to many great

people who made this Masters possible. First I would like to thank my academic advisor

Dr. Hamid M. Lankarani for all his valuable help and guidance. His constant encouragement and

motivation helped me a lot in the completion of this thesis and my masters. In all difficult times

he supported me like a friend and benefactor. I learned a great deal of things from him in my

journey of M.S.

I would also like to thank my committee members Dr. Soschinske and Dr. Krishna

Krishnan for reviewing my report and for their invaluable suggestions to improve my thesis.

Indeed there were very difficult times in performing the finite element analysis where my

friends Prasanna Parvathikar, Arun Gowda and Prasanna kumar Bhonge helped me.

I wish my thanks to Kannan, Shashi, Uma, Amar, Vikas, Arun for their support, moral

boosting and caring. Finally my grateful thanks to my parents, my sisters who are source for

emotional peace and encouragement throughout my entire life.

v

ABSTRACT

Response of a material impacted by projectiles especially bullets, or blast fragments, is

extremely important in determining the range of impact it can sustain. As explicit finite element

codes improve and advances material models become available, the hydrocodes find more

widespread application in many industries. In this thesis, a study of ballistic response is

implemented using simulation of thin metal targets in LS -DYNA. Parametric studies are

conducted to study the effects of various factors on the damage process. Further in the study an

attempt has been made to study the response of composite targets to the projectile impact. For

the composite target, a finite element model is implemented with Chang-Chang failure criteria.

Comparisons of the finite element simulations to the experimental data include general as

well as the time history response. Results indicate that the residual velocities from the

experimental tests correlate well with the ones from finite element validation.

A parametric study is then conducted with the validated models. Parameters including as

projectile velocity, projectile mass, projectile geometry boundary conditions, target thickness

target yield strength, target failure strain and friction between the target and the bullet are

considered, which affect the Ballistic Impact process.

This study demonstrates the accuracy and effectiveness of the finite element simulation

of the impact tests on thin metallic targets with the help of Finite Element softwares.

vi

TABLE OF CONTENTS

CHAPTER PAGE 1. INTRODUCTION.................................................................................................................1

1.1 Introduction Armor systems.......................................................................................... 2 1.2 Introduction Body Armors.. 3 1.3 Ballistic Testing...3 1.4 Composites in Ballistic Applications. 5 1.5 Modulus of Fiber-Reinforced composites.. 7 1.6 Background ... 8

1.6.1 Literature Review...9 1.6.1.1 Analytical Models.9 1.6.1.2 Finite element models.10 1.6.1.3 Penetration equations..................................................11

1.7 Overview..13 1.8 Definition of the problem.13 1.9 Scope of this research..14

2. MECHANICS OF PENETRATION..15

2.1 Introduction to Penetration Mechanics15 2.2 Penetration and failure in Metal Targets.15 2.3 Composite failure and damage.18 2.4 Failure Theories for composites...19

3. FINITE ELEMENT FORMULATION23 3.1 Introduction to FE codes...23 3.2 Time integration24 3.3 Classification of loading25 3.4 Lagrangian Approach27 3.5 Solid Element Formulation... 28

4. FINITE ELEMENT MODELING............ 29 4.1 Modeling details.. 29 4.2 Finite Element Models of Target and Projectile.. 30 4.3 Material Properties for Metal Plate and Projectile. 32

4.3.1 Dimensions of Quarter Symmetry Model 32 4.4 Composite Modeling...................................................... 33 4.5 Material Models 36

4.5.1 MAT_PLASTIC_KINEMATIC.36 4.5.2 MAT_RIGID...37 4.5.3 MAT_COMPOSITE_DAMAGE37 4.5.4 INITIAL_VELOCITY_RIGID_BODY.37

4.6 Modeling Contact..... 37 4.7 How Contact Works.. 38

4.7.1 CONTACT_ERODING_SURFACE_TO_SURFACE..38 4.8 CONTROL_TIMESTEP...38 4.9 CONTROL_CONTACT. 39 4.10 DATABASE_BINARY_D3PLOT.. 39

vii

TABLE OF CONTENTS (CONTD)

CHAPTER PAGE 4.11 CONTROL_HOURGLASS.. 39

5. RESULTS AND DISCUSSIONS.. 40 5.1 Validation. 40 5.2 Parametric study41

5.3 Validation cases43 5.3.1 Validation case 1. 43 5.3.2 Validation case 2.... 45 5.3.3 Validation case 3..................................................... 47

5.4 BALLISTIC LIMIT. 49 5.5.1 Case: Projectile mass: 0.00259kg..... 51 5.5.2 Case: Projectile mass: 0.003239kg.. 53 5.5.3 Case: Projectile mass: 0.003887kg.. 55 5.6.1 Case: Projectile velocity: 1200 m/s... 57 5.6.2 Case: Projectile velocity: 1250 m/s.. 59 5.6.3 Case: Projectile velocity: 1300 m/s. 61 5.7.1 Case: Sphere Radius: 0.003797 m. 63 5.7.2 Case: Sphere Radius : 0.00508 m.... 65 5.8.1 Case: Spherical Projectile velocity: 1115.873m/s...67 5.8.2 Case: Sphere Projectile Velocity: 1200m/s ................................................................................................ 69 5.8.3 Case : Spherical Projectile velocity: 1250 m/s.71 5.9.1 Case: Failure strain of plate 1.75.....73 5.9.2 Case: Failure strain of the plate 1.8075 5.9.3 Case: Failure strain of the plate 1.9085 5.10.1 Case: Composite Impact projectile velocity 125 m/s...87 5.10.2 Case: Composite Impact projectile velocity 187 m/s..90 5.10.3 Case: Composite Impact projectile velocity 200 m/s... ..92

6 CONCLUSIONS AND RECOMMENDATIONS..96 REFERENCES. 99

viii

LIST OF FIGURES

FIGURE PAGE 1.1 Schematic test arrangement for Ballistic test 3 1.2 Example of particle reinforced composite 6 1.3 Fire orientation in fiber reinforced composites 6 1.4 Tensile strength of fibers in longitudinal and transverse direction of a uni-directional fiber composite 6 1.5 Structural composite 7 1.6 Woven fiber structures 8 2.1 Common failure occurring in projectile impact 16 2.2 Rigid projectile impacting a composite 19 2.3 Schematic of failure modes at different depths of the laminate A, B, C represent

the transverse shear, tensile and delaminating regions of the impacted composite 22 3.1 Graph showing load rise time 25 3.2 Unreformed and deformed shading in Lagrangian coordinate systems 27 3.3 Eight node hexahedron solid element 28 4.1 Quarter model of AL 2024 T-3 plate with one way biased meshing 31 4.2 Quarter model of cylinder with butterfly meshing 31 4.3 Quarter model with symmetric boundary conditions 32 4.4 8 Ply Composite Laminate 34 4.5 One way Biased Meshing of the plate 34 4.6 Meshed Projectile 35 5.1.1 Plate deformation 47 5.1.2 Residual velocity of the Bullet 47 5.1.3 Kinetic energy lost by the bullet 48 5.1.4 Internal energy rise in the plate 48 5.2.1 Plate Deformation 49 5.2.2 Residual Velocity of the projectile 50 5.2.3 KE lost by bullet 50 5.2.4 IE rise in the plate 51 5.3.1 Plate deformation 51 5.3.2 Residual Velocity of Bullet 52 5.3.3 KE lost by bullet 52 5.3.4 IE rise in the plate 52 5.4.1 Plate deformation 53 5.4.2 Residual velocity 54 5.4.3 KE lost by projectile 54 5.4.4 KE gained by plate 55 5.5.1 Plate Deformation 55 5.5.2 Residual velocity of bullet 56 5.5.3 KE lost by bullet 56 5.5.4 IE rise in the plate 57 5.6.1 Plate Deformation 57 5.6.2 Residual velocity of projectile 58 5.6.3 KE lost by projectile 58 5.6.4 IE rise in the plate 59 5.7.1 Plate deformation 60 5.7.2 Residual velocity of bullet 60

ix

LIST OF FIGURES (CONTD)

FIGURE PAGE 5.7.3 KE lost by bullet 60 5.7.4 IE rise in the plate 60 5.7.5 Residual Velocity Variation with Projectile Mass 61 5.8.1 Plate deformation 62 5.8.2 Residual velocity of bullet 63 5.8.3 KE lost by bullet 64 5.8.4 IE rise in the plate 64 5.9.1 Plate deformation 64 5.9.2 Residual velocity of bullet 65 5.9.3 KE lost by bullet 65 5.9.4 IE rise in the plate 66 5.10.1 Plate deformation 66 5.10.2 Residual velocity of bullet 67 5.10.3 KE lost by bullet 67 5.10.4 IE rise in the plate 68 5.10.5 Variation of Residual Velocity with Incident Velocity 68 5.11.1 Plate deformation 69 5.11.2 Residual velocity of projectile 69 5.11.3 KE lost by projectile 70 5.11.4 IE gained by the projectile 70 5.12.1 Plate deformation 71 5.12.2 Bullet Velocity vs Time 72 5.12.3 Bullet KE vs Time 72 5.12.4 Plate IE vs Time 73 5.12.5 Variation of Residual Velocity with Sphere Diameter 73 5.13.1 Plate deformation 74 5.13.2 Bullet velocity vs Time 75 5.13.3 Bullet KE vs Time 75 5.13.4 Plate IE vs Time 76 5.14.1 Plate deformation 76 5.14.2 Bullet Velocity 77 5.14.3 Bullet KE vs Time 77 5.14.4 Plate IE vs Time 78 5.15.1 Plate Deformation 78 5.15.2 Bullet velocity vs Time 79 5.15.3 Bullet KE vs Time 79 5.15.4 Plate IE vs Time 80 5.15.5 Variation of Residual Velocity with Incident Velocity 80 5.16.1 Plate Deformation 81 5.16.2 Residual Velocity of Projectile 81 5.16.3 KE Lost by Projectile 82 5.16.4 KE Lost by projectile 82 5.16.5 IE gained by the Plate 78 5.17.1 Plate Deformation 83 5.17.2 Residual Velocity of Projectile 83 5.17.3 KE Lost by Projectile 84

x

LIST OF FIGURES (CONTD)

FIGURE PAGE 5.17.4 IE gained by the Plate 84 5.18.1 Plate Deformation 85 5.18.2 Residual velocity of projectile 85 5.18.3 KE lost by projectile 86 5.18.4 IE gained by the Plate 86 5.18.5 Variation of Residual Velocity with Failure Strain 87 5.19.1 Plate Deformation 87 5.19.2 Delamination of Plies 88 5.19.3 Residual Velocity of the Projectile 88 5.19.4 KE lost by the Projectile 89 5.19.5 IE gained by plies 89 5.20.1 Plate Deformation 90 5.20.2 Delamination of Plies 90 5.20.3 Residual Velocity of the Projectile 91 5.20.4 KE lost by the Projectile 91 5.20.5 IE gained by plies 92 5.21.1 Plate Deformation 92 5.21.2 Delamination of Plies 93 5.21.3 Residual Velocity of the Projectile 93 5.21.4 KE lost by the Projectile 94 5.21.5 IE gained by plies 94 5.21.6 Variation of Residual Velocity with Incident Velocity 95

xi

LIST OF TABLES

TABLE PAGE 4.1 Material properties of AL 2023 T-3 32 4.2 Material properties of Tool Steel 33 4.3 Dimensions of AL 2024 T-3 Plate 33 4.4 Dimensions of Tool Steel Projectile 33 4.5 Material properties Polypropylene/E-Glass 35 4.6 Materials properties of Tool Steel 36 4.7 Dimensions of Single ply 36 4.8 Dimensions of Projectile 36 5.1 Case: Analyzed with FEA and compared with experimental results 40 5.2 Case: Velocity variations 41 5.3 Case: Projectile mass variation 41 5.4 Case: Spherical projectile mass variation 42 5.5 Case: Failure strain variation 42 5.6 Case: Projectile residual velocity variation for composite plate impact 42

xii

LIST OF ABBREVIATIONS

ABBREVIATION DESCRIPTION

FEA Finite element Analysis CD Component Dysfunction KE Kinetic Energy IE Internal Energy

xiii

CHAPTER 1

INTRODUCTION

High velocity impact is of interest to many different fields and has been the subject of

much research, especially in the last 50 years. Over this period of time, the methods used to

analyze impact have changed dramatically, as have the disciplines interested in these

analyses. Researchers are still trying to get a clear cut picture of the impact behavior. Mainly

this applies to the defense industry. Armor resilience and impact resistance are extremely

important in warfare applications.

Many theories and procedures emerged to study the impact and blast phenomena.

Blast phenomena leads to fragment evolution which in turn leads to impact. In space travel

applications impact plays a vital role in designing the sacrificial shield against the debris.

Latest innovations like friction stir welding and repair require the data of impact to read the

impact event to exactly assess the damage and repair parameters. Low velocity impacts can

cause severe damage to soft material like muscle tissue. In early days metals armors were

used, now with advent of composites light weight armor materials are introduced which are

more portable. Lighter materials increase the mobility and portability.

1.1 Introduction to Armor Systems

Military systems especially supporting the ground forces are being transformed to

move faster, more agile and more mobile as to counteract the warfare tactics. Bomb attacks

on armored vehicles claimed lives of Defense troops. As a result, an increased demand for

improved armor has led to the development of new armor materials. Already in some fields

Polymer Matrix Composites, Ceramics and Metal mobility. Research is still going on in this

field to completely replace the armor shield with composite materials which offer good

strength to weight ratios.

1

1.2 Introduction to Body Armors

Throughout history, lightweight and flexible materials have been sought to reduce the

weight of body armor systems to enhance mobility, while providing protection against

specified threats. Early materials included leather and even silk, which were used in

conjunction with metal plates to provide the needed protection in making vests. These vests

provided protection against bomb and grenade fragments, which accounted for the high

majority of injuries and deaths among soldiers. Although nylon and E-glass fibers continue to

find some use today due to their low cost, high performance fibers are now the standard for

most fiber reinforced armor applications. High performance fibers are typically used in the

form of woven fabrics for vests and for helmets. Figure 3 shows the Interceptor vest and

composite.

1.3 Ballistic Testing Impact studies are performed by civil aviation firms concerned with turbine blade

containment; by spacecraft designers concerned with the effects of space debris; and by

survivability analysts concerned with protecting aircraft or other vehicles from man-made

threats. The interests and needs of this last group are the primary motivation for this work.

The job of vulnerability analyst is to determine the vulnerability of a system, such as an

aircraft, to a wide array of threats and work to mitigate the effects of these threats. An

important measure of vulnerability is the probability of kill given a hit (Pk/h), which is

evaluated on a system or aircraft level and probability of a component dysfunction given a hit

(PCD/H) which is determined for a single component. If the threat is taken to be some type of

projectile, then PCD/H is, among other things, a function of projectile mass and velocity. Thus,

if several components lie on a particular shot-line, then the mass and velocity of the projectile

at impact must be known for each component along that shot line. This can be done using

experiments, analytical models, empirical penetration equations or a combination of any of

2

these methods. The majority of design level vulnerability analyses are performed using

penetration equations embedded within higher level vulnerability models. Though each of the

methods for determining projectile residual velocity and mass has certain benefits, they each

have limitations as well.

The limitations of experiments involving impact are obvious. Because they are by

design destructive tests, they can be costly to perform, in terms of materials, labor and time.

Furthermore, they are somewhat stochastic by nature, making it difficult to repeat any given

experiment or apply the results to a vulnerability analysis. A schematic arrangement of test

setup for projectile impact is shown in Figure 1.1.

Figure 1.1 Schematic test arrangement for ballistic test [1]

Most common method for assessing the lightweight armor materials for ballistic performance

is by placing a witness plate behind the armor panel which determines the outcome of the

ballistic test as shown in the Figure [1].

Complexity involved in measurement increases with velocity. Ballistic events are

commonly performed using powder gun which is similar to the gas gun, but makes use of gun

powder instead of gas to propel the bullet. Ideally one would be able to measure the projectile

3

displacement or velocity during an impact event. While the analytical models are physics-

based, they use simplifying assumptions in order to reduce the governing equations to one-

and two-dimensional equations. These models also only look at one aspect of the problem,

and are not capable of examining every possibility or aspect of a complex penetration

problem [1].

Empirical equations, also referred to as penetration equations, are extremely valuable

because of their simplicity and ease of use, but they also have shortcomings. First, they are, in

essence, curve-fits of experimental data and are therefore limited to the range of conditions

and quality of results of the experiments. Secondly, as mentioned above, experimental results

are not necessarily precise, and it is not feasible to conduct a real-world impact experiment

for every possible scenario that might be encountered, thus limiting the databases from which

these equations are created.

With the ever increasing power and speed of computers, and the refinement of finite

element (FE) codes and explicit dynamic solvers, it is possible to use numerical analysis and

computer simulation to model ballistic impact events. Once a model is created, simulation

results can be compared with available experimental test data, and the FE model can be

refined until the user is confident of the results generated by the simulation. Certain FE

modeling parameters, such as material properties at high strain rates, depend on experimental

data, but since the FE simulations are not based on curve-fits to impact test data, simulation

results are not affected by possible experimental error in some trials in a set of test data.

Because of this, there can be greater confidence in the FE results, compared to penetration

equations, in regions where test data is not available. FE simulations can be used to model

impact experiments before they are performed, in order to reduce cost and increase

efficiency. They can also be used to augment and refine the existing penetration equations,

filling in gaps where experimental data does not exist or is insufficient.

4

A projectile is considered compact if it is in the shape of a cube, parallelepiped or

cylinder, with a length-to-diameter ratio (L/D) of approximately one. A real world scenario

which would include compact projectiles is a missile warhead detonating external to an

aircraft, where the fragments from the warhead can be modeled as compact projectiles and

the aircraft components as flat plates. In this work, the PATRAN pre-processor, and the LS-

DYNA explicit dynamics solver, is used to model the above scenario. The residual velocity

of the fragment is determined from the simulation and also ballistic limit was found. The

results of these computer simulations are then compared to experimental data, as well as

predictions from two sets of penetration equations. A more complete presentation of the

analyses and results can be found in [2].

1.4 Composites in Ballistic Applications

Composites on the offer very high strength to weight ratios and are hot favorites in

aviation and other fields where light weight components that offer high endurance are

desired. Composite materials unlike metals lose structural integrity and strength to a great

extent upon impact. Composites are combinations of two or more materials embedded in

another material called matrix. The reinforcing material can be metal, ceramic or polymer.

The combination offers properties superior to individual components. The orthotropic

property of composite allows us to design to our requirements still keeping the overall weight

minimum. High strength to weight ratio, High creep resistance, High tensile strength, and

High toughness are main factors behind the use of composites in many applications.

Three types of composites are:

1. Particle-reinforced composites (as shown in figure 1.2)

2. Fiber-reinforced composites (as shown in figure 1.3)

3. Structural composites ( as shown in figure 1.4 )

5

Figure 1.2 Examples of Particle Reinforced Composites [2]

Figure 1.3 Fiber orientation in fiber reinforced composites [2]

Figure 1.4 Tensile Strength of fibers in longitudinal and transverse direction of a uni-directional fiber composite [2]

6

Figure 1.5 Structural composites [2]

1.5 Modulus of Fiber-Reinforced Composites:

Fibers have a very high modulus along their axis, but have a low modulus

perpendicular to their axis. If the fibers are all parallel, the modulus of a fiber reinforced

composite depends upon which direction you're measuring. The modulus of the entire

composite, matrix plus reinforcer, is governed by the rule of mixtures when measuring along

the length of the fiber:

Ec = EfVf + Em (1.1)

Ec is the modulus of the entire composite along the length of the fiber.

Ef is the modulus of the fiber along the length of the fiber.

Vf is the volume percent occupied by the fibers.

Em is the modulus of the matrix (usually not dependent upon direction)

Vm is the volume percent occupied by the matrix (equal to (1-Vf)).

High performance fibers typically used in the form of vests and either woven or non-

woven reinforcements within polymer matrix composite for helmets in defense. Polymer

7

matrix composites are now slowly substituting the places where metals are heavy to use.

Fibers can be woven into a number of configurations, some of which are illustrated in Figure

1.1. Fibers for armor applications have traditionally been in unidirectional, plain or basket

weave composites. Woven structures have been studied to enhance the multi-hit capability of

the composites.

Figure 1.6 Woven Fiber Structures [7]

Low velocity impacts are found to cause matrix cracking, fiber breakage and

delamination. High Impact in composites generally causes little global structural response

and more of local deformation as shown in Figure 5. In general there are many parameters

that define the damage nature in composite structures, such as delamination, which is

sensitive to compression loadings. Therefore study of the parameters affecting the damage in

impact is important.

1.6 Background and Literature Review

The experimental work in this research focuses on compact steel projectile impacting

aluminum target with low range velocities. A projectile is considered compact if it is in the

shape of a cube, parallelepiped or cylinder, with a length-to-diameter ratio (L/D) of

approximately one. A real world scenario which would include compact projectiles is a

missile warhead detonating external to an aircraft, where the fragments from the warhead can

be modeled as compact projectiles and the aircraft components as flat plates called as

Fragment Simulation Projectiles. The study of high velocity impact is of importance to many

8

fields, and it is a topic that has been studied for many years, especially following World War

II. As a result, there is an abundance of high-velocity impact models.

These models can be divided into several different categories based on two types of

criteria. First is the type of model, which is analytical, numerical or empirical, though

empirical models may incorporate elements of analytical analysis. In the context of this work,

empirical models are synonymous with penetration equations and will be discussed below.

The second criterion is the type of impact being modeled, and this can be categorized based

upon projectile size, shape or material, target material or thickness, or the velocity at impact.

In terms of projectile shape, these are generally classified as blunt, such as cylinders or cubes,

or pointed, such as ogival or spherical. The size of the projectile is based upon either the mass

or the dimensions, such as the length to diameter ratio, or a combination of both factors.

Target thicknesses are generally classified as thin, which have a thickness less than or equal

to the projectile diameter; moderately thick, which is generally up to several times the

projectile diameter; or semi-infinite, where total penetration is assumed to never occur. In this

present analysis work validation is done for three cases of different target thickness and L/D

ratio.

1.6.1 Analytical Models Some of the earliest analytical models were developed for moderately thick targets

impacted by rigid projectiles, the simplest of which are one-dimensional and one stage and

are derived from energy and momentum balance equations [3]. Awerbuch and Bodner [4]

refined the one-stage model into a three-stage, one-dimensional model. This model, coupled

with the one-stage model equation, can be used to determine the residual velocity of the

projectile. However, it is only applicable to thick targets and rigid projectiles. Later, Ravid

and Bodner [5] published a five American Institute of Aeronautics and Astronautics 3-stage,

two-dimensional model. The main differences between the five-stage and three-stage models

9

are that the five stage model eliminates physical ambiguities and empirical factors and allows

for target failure modes other than plugging.

1.6.2 Finite Element Models

With the widespread use and increased power of computers physics-based numerical

analyses of impact problems has become possible. Examples of numerical methods used are

the finite difference and the finite element methods, either using an Eulerian (fixed) or

Lagrangian (deformable) mesh. Currently the most widely used codes are finite element with

Lagrangian meshing [6]. While there have been many numerical analyses of impact, they

typically involve either low velocities (1000 fps or slower), hypervelocity impact (beyond

10,000 fps), non-blunt projectiles, long rods, or penetration but not perforation of the target.

A series of impact and penetration simulations were performed by Sedgwick et al in 1978

using the HELP 2-dimensional Eulerian continuum mechanics code. Impact between steel

cylindrical projectiles impacting thin aluminum plates was modeled. At high velocities the

residual velocities predicted by the model compared well with experimental results, but

experimental data scatter at lower velocities impaired accurate comparisons [7]. In 1984,

Hallquist [8] conducted a simulation of impact between a rigid sphere and a thin elastic-

plastic plate using DYNA-3D. No experimental data was published, but the failure

mechanism for the plate functioned correctly. Chen [9] performed a series of eight tests in

1989 to verify that a Langrangian code, PRONTO-2D, could accurately predict the residual

velocity of a conical nosed projectile after the penetration of a 2.5 cm thick, 6061-T6

aluminum target. Because the elements used to model the target would not allow the

formation of a hole between elements only a quarter of the projectile and target were

modeled, allowing elements to be pushed aside to simulate penetration. The accuracy of the

simulations was described as good but no actual numbers and percentage errors were

published.

10

In 1990 Bamman [10] used DYNA-2D to predict the ballistic limit of a 6061-T6

aluminum target. The target was 3.2 mm. thick and assumed to be rate and temperature

dependent deviatoric plastic with a failure. Only two cases were conducted, but the results

were described as very accurate. In 1993 Barrett [11] used DYNA-3D to model ballistic

impact involving both aluminum and composite targets and used several different material

models. The residual velocity, number of plates penetrated, hole sizes, size of the plastically

deformed region, the projectile deflection angle, and the post impact attitude of the projectile

were examined. The results of the simulations were compared to experimental data obtained

from tests performed by the Boeing Company in the 1970s. Using a strain-rate dependent

elastic-plastic material model for the target and an elastic-plastic material model for the

projectile, he was able to predict the residual velocity of the projectile with an average error

of 32.0%, where error was defined as the difference between the experimental and simulation

residual velocities, divided by the change in velocity for the experiment. The projectiles used

were mild steel cylinders, with L/D values of between 1.03 and 4.77, and masses of 43 to 400

grains. The initial velocities used were between 537 and 2480 feet per second, with the

majority being less than 2000 fps. The target thicknesses were between 0.032 and 0.375

inches, with the majority of the targets being less than 0.125 inches in thickness. A three-

dimensional Lagrangian FE code was developed in 2002 by Yoo and Lee [12] in order to

analyze large deformations in contact and penetration. Comparisons were made between

experimental data and numerical results for ductile metal spheres and long rods impacting

thin ductile metal plates at high velocities. For the ballistic limit of the plates impacted by

spherical projectiles, the agreement between the simulations and empirical data was poor for

0 obliquity impact, but improved at higher obliquity angles. The long rod (L/D = 15)

comparisons were for very high velocity impacts (< 1 km/s) and the residual length and

velocity agreement between the simulations and empirical tests was very good.

11

1.6.3 Penetration Equations

In general, a penetration equation is a set of equations that are used to predict the

outcome of an impact event, such as the residual velocity or mass of the projectile after

impact. Empirical penetration equations are essentially curve-fits and take the general form

f(x1, x2 xn), where x1, x2 xn are parameters such as projectile size and target thickness. It is

important to note that results of these equations are only accurate if the case for which it is

being used is close to that of the experimental data to which the equations are fit [1]. For this

work, the results of the FE simulations were compared to the predictions of two empirical

penetration equations, THOR [12] and the JTCG/ME equations for kinetic energy penetrators

[14]. Both of these sets of equations are used extensively in the vulnerability community and

are incorporated into higher level vulnerability codes such as COVART (Computation of

Vulnerable Area and Repair Time).American Institute of Aeronautics and Astronautics 4 the

THOR equations were developed under the code name Project THOR in the early 1960s.

For perpendicular impact of a steel projectile, the equation for the residual velocity (Vr) of the

projectile is a function of the projectile mass (M), cross sectional area (A), initial velocity

(Vi), and target thickness (t), where a, b, c, and d are empirical constants.

di

cp

bair VMtAVV )(10= (1.2)

The empirical constants were determined by a least squares fit of the experimental data,

which also included oblique (non-perpendicular) impact. In the late 1970s the Joint Technical

Coordinating Group for Munitions Effectiveness (JTCG/ME) sought to ensure consistency in

the use of penetration equations for aircraft vulnerability analyses. The penetration data and

methodology available at the time was reviewed and analyzed, resulting in the JTCG/ME

Penetration Equations Handbook for Kinetic-Energy Penetrators [15]. For these equations,

for mild steel fragments the residual velocity is a function of the projectile initial velocity and

12

presented area and the target ballistic limit, density and thickness. The ballistic limit in turn is

a function of the projectile mass and presented area, and the target density and thickness, as

well as the angle of obliquity [14].

1.7 Overview

Importance of nature of the Ballistic Impact of both Metal and Composite has been

generally recognized both on Space, Civil Aviation, and Military and Automotive industries.

Heavy metal armors are deployed for very high speed applications and composite materials

are for gaining high strength to weight ratios. Efforts are taking place to replace metals to

save overall weight of the Component. Therefore impact problems become important. A

dropped wrench, bird strike or runway debris can generate localized delaminated areas due to

foreign object damage (FOD). Because of the failure mechanism in composite, there is still

no generally accepted analytical model to predict the impact damage of composite laminates.

The micro failure modes commonly observed in composite laminates are

1. Fiber Breakage

2. Fiber Micro Buckling and Matrix Crushing

3. Transverse Matrix Cracking

4. Fiber Breakage

5. Debonding at the fiber-matrix interface

6. Delamination

The debonding and delamination can only be viewed in three dimensional representations

which were shown in this research.

As Explicit Finite Element codes improve and advanced material models finding

more application in many industries. The ability of the finite element solver to model the

damage that arises from the impact load will provide the suitability and applicability for

composite structures. The derivation of a finite element model for impact is governed by

13

certain behavioral characteristics of the impact process. These damage loads often suggest

dynamic impact as an appropriate choice. Prediction of the Ballistic limit is a very difficulty

task for which complete success may not be possible. Therefore extensive experimental work

is being done to date to understand which parameters affect the impact failure in composite

structures.

1.8 Definition of the Problem

Impact and penetration of a Tool Steel projectile in to AL 2024 T-3 was performed

for the experimental data in [1]. Once the simulation results agreed with the experimental

data a parametric study was conducted to study the effect of different factors on the impact

event.

Further simulations were performed on impact of Tool Steel projectile on

Polypropylene/ E-Glass composite. Material properties were taken from work of Vaidya and

Bartus and Deka [18]

1.9 Scope of this Research

Prior to sophisticated FEA programs, experimental analysis was the instrument used

to examine impacts that exhibited any degree of complexity. Experimental analysis is

expensive and requiring many testing prototypes, test equipment, and test environment. In

high-speed or impact testing, damage or destruction of the prototype is required before

meaningful quantitative information about design can be obtained. A significant advantage of

FEA over the experimental method is the examination of a virtual prototype in a virtual

environment. This allows for a more concurrent analysis of the design during the designing

process, thus reducing engineering costs and testing while increasing product performance.

The understanding of physics involved in impacts is necessary to carry out good numerical

analyses.

14

The scope of this thesis includes the analytical study of high velocity cylindrical

projectile impact on thin metal plates used in vehicle armor applications using explicit finite

element solver LS-DYNA. The simulation results are verified with experimental results.

Ballistic limit or maximum velocity of the projectile that a target can stop with penetration

was found. A parametric study is conducted to find the effects of different parameters like

velocity of the impact, plate thickness, geometry of the projectile, friction, failure strain.

Further a study is conducted on low velocity cylindrical projectile impact of laminated

composite used in body armor applications. Solid eight node hexahedral element with one

point integration was used in both the analysis. The main focus of the study is to provide

comprehensive details on the formulation of impact analysis and parameters affecting the

process.

15

CHAPTER 2

MECHANICS OF PENETRATION 2.1 Introduction to Penetration Mechanics

The penetration mechanics, also known as the impact and penetration mechanics, is

an interdisciplinary subject. A comprehensive discussion of the relevant background would

be quite extensive. However, this thesis focuses on the ballistic response during the impact.

2.2 Penetration and Failure in Metal Targets

Metals are isotropic materials i.e., having same properties in all directions. Models of

penetration and perforations are based on laws of conservation and compatibility. As an

impact occurs, the kinetic energy of the projectile is imparted to the plate. Some of the energy

is used to deform the plate. Other energy is given off as light and heat, the remainder of the

energy is imparted to the fragments as kinetic energy. Measuring or determining each of

these energies is very difficult.

For penetration and perforation analysis, the only important aspect is to predict the

kinetic energy (i.e. mass and velocity) of the fragments. Once this kinetic energy is

determined, conservation of mass and energy, sometimes in terms of momentum, is applied

to the projectile/target system. The analysis is still quite complex because the events that

occur at the projectile/ target interface are somewhat unknown. Although many studies have

been performed, only highly controlled velocities, shapes, sizes and trajectories have been

examined. As a result, numerous approximations and assumptions must be made in order to

apply to these analyses to fragments. Impact is a much localized phenomenon. Stress and

strain effects are usually limited to within 3-6 projectile diameters of the impacted zone [18].

Impacted target materials may fail by a combination of several modes including spalling,

plugging, petaling, ductile or brittle fracture, and adiabatic shearing. Figure 12 shows some of

these failure modes.

16

Figure 2.1 Common failures occurring in projectile impact [3]

A target is considered thick if the distal boundary is influential only after substantial

travel of the projectile into the target. For thin targets distal side responds immediately for

impact on the frontal side. Spalling is tensile failure of the target material due to the reflection

of the initial compressive waves from the far side of the target. Failure by spalling can occur

on either the front or back of a target and is characterized by the formation of petals or ejects.

In ductile failure, the impact impulse overcomes the peripheral dynamic shear strength of the

target material, pushing it outward and toward the impact surface to form a crater that is

much larger than the projectile diameter [21]. At the same time, the projectile pushes into the

17

target, and there is hydrodynamic erosion and inversion of the penetrator material against the

preceding face of the target.

The penetration process due to high-velocity impact can be represented by four

phases: transient, primary penetration, secondary penetration, and recovery [22]. The first, or

transient, phase is characterized by a very short pressure spike and occurs when the projectile

first contacts the target surface. The primary penetration phase is described as the period

during which the projectile acts as a contributing force, imparting its kinetic energy to the

target in a hydrodynamic manner. The secondary phase (more than one phase may occur

simultaneously), sometimes referred to as cavitation, begins after the projectile is completely

deformed and effectively removed from the system as a source of energy. It is marked by

target deformation not caused directly by the KE of the projectile material. Instead, the

energy density behind the expanding shock wave continues to deform the target material. The

fourth, or recovery, phase refers to the period during which the crater recovers or contracts

slightly. Material just below the target surface anneals and re-crystallizes.

Projectile failure occurs simultaneously with target failure. Thus, penetration models involve

both things. The projectiles deform and flatten/spread out as they strike the target, generating

high resisting contact forces. For low L/D ratios, either model gave reasonable predictions.

Expectedly, this also suggests that a combination of both phenomena actually takes place.

Another penetration model is similar to the erosion model, but of a more

hydrodynamic nature. The particular treatment here is taken from [24]. In this model, the

front end of the projectile and the impacted surface are modeled as flowing liquids. The

regions directly behind these surfaces are then modeled as rigid bodies. The projectile is

consumed from the impact end as it penetrates the target material and is transformed into a

Further it predicts that most of the impacted target material is displaced forward and outward

18

by the projectile during penetration and that a small amount is ejected backwards. Maximum

strain criterion is used to show the failure of the material.

In present analysis no data is available regarding the deformation of the projectile and

mass loss of the projectile, so the projectiles deformation is ignored in the target. In the event

of Impact there is an exchange of energy takes place.

19

platetrans KEKEE ++ erodededplate IEIE += (2.2) erod

Law of Conservation is observed in any physical phenomena. Kinetic energy of the

projectile is spent in raising the internal energy and kinetic energy of the plate and some part

of the energy is lost in the form of eroded material. This is described by the equation (2.2),

where E, IE, KE denote total energy, internal energy, kinetic energy, subscripts trans and

plate denote transmitted and related to plate. The superscript eroded denotes eroded mass.

Blunt projectiles like cylinders are found to cause plugging because of pure shear failure,

while the conical projectiles are found to cause petaling effect. The amount of energy

dissipated also differs with the geometry.

2.3 Composite Failure and Damage

Composites are orthotropic materials i.e., having different properties in perpendicular

directions. Parameters which significantly affect the properties of a composite are shape, size,

orientation and distribution of the reinforcement and various other features such as matrix,

grain size in case of polymer matrix composites. These together with volume fraction

constitute what is called the microstructure of the composite. The orientation of the

reinforcement within the matrix affects the isotropy of the system. When the reinforcement is

in the form of equiaxial particles, the composite behaves essentially as an isotropic material

whose elastic properties are independent of direction. Manufacturing process may result in

different orientation of the reinforcement and hence the loss of isotropy; thus composite

becomes anisotropic in nature. High velocity impact will cause localize compression of the

composite and subsequently shearing the fibers and spalling of the resin during impact, the

fibers take the shear loading. Once the projectile has slowed, the composite deforms causing

fiber stretching, pullout, and delamination of the composite layers (plies) and thus lower load

carrying ability.

Figure 2. Rigid projectile impacting a composite [4]

2.4 Failure Theories for Composites

Macro mechanical failure theories have been proposed adapting isotropic failure

theories that account for anisotropy in stiffness and strength of the composites.

a) Maximum stress theory: The maximum stress criterion of the corresponding to the

strength in fundamental failure modes. If any of the limits exceed the corresponding

stress value, material is deemed to have failure when

1 = F1t when 1>0 (2.3)

= -F1c when 10 (2.5)

= -F2c when 1

F2t is the transverse tensile strength

F2t is the transverse tensile strength

F2c is the transverse compressive strength

F6 is the shear strength

b) Maximum strain theory: Unlike the maximum shear stress theory, maximum strain

criterion merely substitutes strain in the above mentioned five criteria. Failure occurs

when strain components along the principal axes exceed the corresponding ultimate

strain I that direction. There fore failure has occurred in the composite laminate when

1 = 1tu when 1>0 (2.8)

= 1cu when 10 (3.0)

= 2cu when 2

5. , nonlinear shear stress parameter

S1, S2, S12 and C2 are obtained from material measurement. is defined by material shear

stress-strain measurements. In plane stress, the strain is given in terms of the stress as

)(1 2111 = E (3.3)

)(1 1222 = E (3.4)

3121212

1212 +=

G (3.5)

Where , , , denote Strain, Principal stress, Poissons ratio, Shear stress and subscripts

denote the principal directions. The third equation defines the nonlinear shear stress

parameter

The fiber matrix shearing term augments each damage mode:

4

1212

212

412

12

212

43

2

43

2

SGSG

+

+= (3.6)

Failure is assumed whenever

+

+

=

2

22

12

22

12

2matrix 122

FCSS

(3.7)

Failure is assumed whenever Fcomb>1. If Fcomb>1, then the material constants E2, 1, 2 are

set zero.

Very little work was performed in the development of a numerical model for fiber-

reinforced layered composites. Therefore further study on composite targets was

conducted to study the response in ballistic impact event. Unlike metals, composites lose

structural integrity and strength with an impact. A key element in this development effort

was in identifying and quantifying the different failure modes as the projectile penetrates

22

the composites. A schematic of these processes is shown in Fig. 2. The initial penetration

zone is dominated by punching shear failure, followed by ply tensile failure and then

delamination.

Figure 2.3 Schematic of failure modes at different depths of the laminate A, B, C represent the Transverse Shear, Tensile and Delamination regions of the

impacted Composite [5]

23

CHAPTER 3

FINITE ELEMENT FORMULATION

3.1 Introduction to FE Codes

Today good numbers of FE codes are now available in commercial market that are

capable of performing challenging engineering problems making use of the advanced

computational capabilities offered by modern day processors. Some of the popular FE

processors are LS-DYNA, MSC DYTRAN, MSC NASTRAN, ABAQUS, ANSYS, MSC

MARC, COSMOS, I-DEAS. Pre-processors like MSC PATRAN, HYPERMESH and

MENTAT are capable of generating finite element models for the codes mentioned above.

Apart from performing they are capable of general post processing and time history

processing.

In current analysis MSC PATRAN is used as main pre-processor LS-PREPOST

which has options for adding the cards for preparation of the code for processing in

LS-DYNA which is the processor and LS-PREPOST as the post processor.

Finite element analysis involving short-time large deformation dynamics such as

crashworthiness evaluation requires the solution of transient dynamic problems over a short

time length. Explicit and implicit solution techniques or a combination of both have been

used as the basis for FE crash codes. Explicit computational algorithms typically used the

central difference method for integration, wherein the internal and external forces are

summed at each node point, and a nodal acceleration is computed by dividing by the nodal

mass. The solution is advanced by integrating this acceleration in time.

The implicit method uses the Newark forward difference method for integration [22],

whereby a global stiffness matrix is computed, inverted, and applied to the nodal out-of

balance forces to obtain a displacement increment. The advantage of this method is that time-

step size may be selected by the user. The disadvantage is the large numerical effort required

24

to form, store, and factorize the stiffness matrix. The major practical difference between the

explicit and the implicit solution technique is the requirement on the time step size, t.

The explicit solution technique is stable only if time-step t is smaller than tcr (tcr

is the critical time step for shell elements, is given by tcr =Ls / C, where Ls is the

characteristic length and c is the speed of sound, C = )1(/ 2 E ). The implicit 45 method is not bound by the time-step size and is therefore unconditionally stable for larger time steps.

Hence an implicit solution typically involves a large number of expensive time steps.

Although the number of time steps required for an explicit solution can be larger than that of

implicit methods, the small time-step size requirement makes the explicit method suitable for

short transient solutions. The major advantage of the explicit method is that there is no

requirement for solving simultaneous equations, which means that no global matrix inversion

is required, thus reducing computational time.

3.1.1 Time Integration

High-speed/impact is certainly a dynamic event. Time integration routines are

required in numerical analysis to solve for accelerations, velocities, and displacements of the

dynamic problem, characterized by the system equation:

),(22

utFKuudtdM =+ (3.1)

Where M is the system mass matrix, K is the system stiffness, and u is the system

displacement vector to a load vector of F. The time-step method may be classified as either

explicit or implicit. Explicit methods are usually used in central deference, while implicit

methods are usually incorporated into FE analysis. In an explicit scheme, the next time step

of nodal displacement u can be determined by the preceding time steps of displacements.

Using central difference equations, the velocity and acceleration are expressed as

)(1

11 jjj uutu

dtd = ++ (3.2)

25

][21

112

2

+ = jjj udtdu

dtd

tu

dtd (3.3)

Where j is the current step, j+1 is the next step, and j-1 is the previous step in time. t

is the increment between time steps. Substitution of the current time step j for the velocity

and acceleration from equations (3.1) and (3.2) yields an equation for the displacement at the

next time step J+1 of

(3.4) 122

1 )2( + += jjjj MuuKtMFtMu

With uj+1 known, the j+1 velocity can be known and the j acceleration determined between

the past data value (j-1) and the future data value j+1. A careful time step-size must be

selected in order to provide stability to explicit algorithms. Usually LS-DYNA calculates the

time step-size automatically. The time step-size should decrease in order for the solution to

be stable.

Figure 3.1 Graph showing load rise time [6]

3.2 Classification of Loading

Four classification of loading are generally recognized in engineering: is static,

fatigue, high-speed/rapid loading and impact or shock. These classifications are categorized

by the rate of loading or the rise time upon the mechanical System or component. Figure 15

shows the diagram that defines the load rise time on a system. Static and Fatigue Loading:

26

Static loading occurs when the rise time of the load is three times greater than the

fundamental period (Tn) of the mechanical system. The usual methods of analyses of stress,

strain, and displacements along with static material properties are used to analyze the system.

Fatigue loading is a time-varying load whose rise time from one magnitude to another

magnitude still remains greater than three fundamental periods.

High Speed or Rapid Loading: This occurs when the rise time of load applications

ranges between 1.5 to 3 times the fundamental periods of the mechanical system. Vibration

methods of stress and deflection analysis should be used in the loading category. Impact

Loading: If the time of load application is less than 0.5 times the fundamental period of the

mechanical system, the loading is defined as impact. The static methods of stress, strain, and

deflection analysis are meaningless under impact conditions. This is due to propagation,

reflection, and interference of elastic/plastic waves traveling within the engineering solid.

Accurate calculations of stresses and strains most of be based on wave analysis methods,

which are exceedingly complex for practical use, and thus must be solved for a limited

number of simple cases. Other methods such as contact mechanics, energy methods, and FEA

must be used to estimate the effects of impact analysis on mechanical systems that exhibit

complexity.

Reasons for using the FEA Method in High Speed and Impact Loading conditions are

analytical methods are useful in making predictions and understanding the dominant features

of impact problems, given the engineering problem can be simplified to a simple geometry.

Thus, geometry complexity limits the use of analytical methods.

In general, high-speed/impact problems present a complexity of geometry, stiffness,

mass distribution, impact angle, contact areas, and multiple impacts. In these cases, the only

tool for complex analysis of impact or high-speed is some form of numerical methodology.

Two classes of numerical methods exist for the analysis of impact problems- the finite

27

difference method and the finite element analysis method. The finite difference method has

the advantage of examining hypervelocity (high velocity) impacts involving severe damage

or plastic flow and analogous to fluid flow/elastic deformation. FEA is applicable to slower-

impact scenarios and as the advantage in addressing irregular geometries and boundary

conditions.

3.3 Lagrangian Approach

In Lagrangian coordinate system the coordinates move with the material, it is suitable

for following the regions of relatively low distortions and possibly large deformations. The

Lagrangian coordinate system will deform with material and therefore accurately define

material interfaces as shown in figure (3.2) below. The history of the state of the material in a

cell is known completely. Compared to the Eulerian method the Lagrange method tends to be

faster computationally as no transport of the material through the mesh needs to be calculated

thus saving computation time. Draw back in Lagrangian formulation is excessive distortion

leading to much smaller time steps. But using proper element deletion criteria the advantages

of Lagrangian formulation can be utilized.

Figure 3.2 Undeformed and Deformed shading in Lagrangian coordinate systems.

Different colors represent different materials. [7]

Other Approaches of Formulation

28

Other popular methods of formulation are Eulerian, Discrete Lagrangian formulation and

Smooth Particle Hydrodynamics. Eulerian meshes are stable because they can sustain large

deformation and also flow calculation is possible. But need a very fine mesh, the

computational cost is high compared to Lagrange and also materials borders are unclear.

Compared to the Eulerian method the Lagrange method tends to be faster computationally as

no transport of the material through the mesh needs to be calculated thus saving computation

time. Discrete element method can be efficient, but the computation cost is very high because

breakable spotwelds should to be defined. Smooth Particle Hydrodynamics approach

produces a better result but the final state of the failed element cannot be known. It doesnt

have tensile stability. So it can be concluded that the Lagrange formulation with effective

plastic strain can be the best of the choices with least computation cost for high speed

impacts.

3.4 Solid Element Formulation

Figure 3.3 Eight node hexahedron solid element [6]

29

Single point integration solid is used in the element formulation to save computational time

which is not possible in case of fully integrated solids. Fully integrated solids may be used in

the case of materials with higher Poissons ratios.

30

CHAPTER 4

FINITE ELEMENT MODELING OF PROJECTILE IMPACT MODEL

4.1 Modeling Details

In this analysis the plate material is AL2024 T-3 projectile material is Tool Steel.

Actual plates dimensions are not available so preliminary runs were conducted to model the

plate to exactly behave as in real world scenario. To understand the effect of L/D ratio

experiments were run for different thicknesses and L/D ratios [1].The target is a square plate

and the bullet is a cylinder. The actual dimensions of the AL 2024 T-3 plate are not provided

in the experimental data. Finite element model is prepared in PATRAN and key file is

generated for LS-DYNA. In impact event the damaged area is localized so one way biased

meshing is used. Experimental can be obtained from [1].

So preliminary analysis runs were conducted to find out the effect of plate dimensions

and constraints. As the event is high speed one it has been found that the boundary conditions

have negligible effect. But even then boundary conditions are not found to contribute towards

the failure results. Reduction in the plate dimensions and symmetric boundary conditions

reduced the computation time. Since the impact is much localized, one way biased meshing is

implemented which allows dense in the impacted region and coarse mesh at the edges saving

computation cost. The cylinder is modeled by extruding the butterfly meshed circular lamina.

The problem can be also modeled with shell modeling approach with through

thickness integration points. Though shell modeling approach provides details of transverse

loading phenomena, it cannot exhibit transverse deformations in out-of-plane loading. Solid

modeling approach (hexagonal solid element) is used in modeling both the target and the

bullet so that it shows exact through thickness deformation and realistic view of the event.

Single point element formulation is used as it is much stable. Moreover the model doesnt

contain any materials with Poisson ratio close to 0.5, which eliminates the need for fully

31

integrated solid formulations. Lagrangian 3-D codes are very effective for analyzing

penetrations and deformations. So Lagrangian approach is being used in our present case to

study the deformation that is occurring during the impact.

Although there is no experimental data is available to compare stresses generated

during impact to those given by the simulations, stress plots from the simulation do provide

some validation that FE model created is behaving as expected. Plots from the stress strain

curves show stress waves being propagated to edges and then reflected back towards the

center of the target. In this analysis rigid body formulation is used for the projectile No

deformations are taken into consideration so density of the material is the only thing that

plays an important role as the density is related to mass. Hence just varying the density we

can vary the mass of the projectile.

4.2 Finite Element Models of AL2024 T-3 Target and Tool Steel Projectile

In order to save computational time and to take advantage over symmetry of the target

and the projectile are modeled as quarter models by invoking symmetric boundary

conditions. Since the impact is much localized the impacted region is meshed densely and

rest is meshed coarsely with the help of one-way biased technique, this saves a lot of

computation time. Through thickness meshing is kept uniform. Proper care is taken to

maintain lesser aspect ratio. Initially a 2-dimensional mesh is generated and swept along the

normal direction.

In the figure 4.1 one way biased meshing is shown. Proper care was taken to maintain

aspect ratio less than 5. In figure 4.2 butterfly meshing is shown. Projectile-Plate impact

model with symmetric boundary conditions

32

Figure 4.1 Quarter model of AL 2024 T-3 plate with one way biased meshing

Figure 4.2 Quarter model of cylinder with butterfly meshing

33

Figure 4.3 Quarter model with symmetric boundary conditions

4.3 Material Properties and Dimensions of the Metal Plate and Projectile

Table 4.1describes the properties of AL 2024 T-3, the plate material. The tangent modulus in

the table is used to account for the bi-linear behavior of the material.

Table 4.1 Material properties of AL 2024 T-3

Density, 2780 kg/m3

Youngs Modulus, E 73.1E9 Pa

Poissons Ratio, 0.3 Tangent Modulus, Etan 1.47E9 Pa

Yield Strength, 345E6 Pa

Table 4.2 describes the material properties of the projectile, Tool Steel.

34

Table 4.2 Material properties of Tool Steel

Density, 7924 kg/m3

Youngs Modulus , E 210E9 Pa

Poissons Ratio, 0.28

Table 4.3 describes the geometric detail of the Plate.

Table 4.3 Dimensions of AL 2024 T-3 Plate

Length 82.5 mm

Width 82.5 mm

Thickness 3.175 mm

Table 4.4 describes the geometric details of the Projectile, L/D denotes the length to diameter

ratio of the cylinder.

Table 4.4 Dimensions of Tool Steel Projectile

Diameter (mm) 7.5946 mm

L/D 0.713

4.4 Composite modeling

Similar to AL 2024 T-3 plate the composite plate is also modeled in PATRAN the

key-file is generated for LS-DYNA. The Ply to Ply contact is defined using AUTOMATIC

CONTACT ALGORITHM with friction equal to 0.1. A [90]s, which symmetric layup of

alternating 0 and 90 plies was used. The material models used for composite

MAT_COMPOSITE_DAMAGE does not support failure and deletion of the elements from

the calculation. This results in sever distortion of the elements and fall in time step size.

Sometimes it might result in termination of calculation as the software cannot decrease the

time step anymore. In order to overcome this problem MAT_ADD_EROSION feature of LS-

DYNA is used this helps in removal of the elements that are approaching element distortion.

35

The figure 4.4 shows the eight plies of the composite laminate in a sequence.

Coloration is given to each ply to differentiate between individual plies.

Figure 4.4 8 Ply Composite Laminate Figure 4.5 shows fine meshing of the impacted region and coarse meshing at the

edges.

Figure 4.5 one way biased meshing of the plate

36

Figure 4.6 Meshed Projectile

Figure 4.6 shows the meshed model of the projectile with butterfly meshing.

4.5 Material Properties and Dimensions of Composite Plate and Tool Steel Projectile

Material properties of Polypropylene/E-Glass composite are shown in table 4.5, XT, YT, ZT ,

denote the tensile strength in X, Y, Z directions, Yc denotes the compressive strength in Y

direction and SC denote the shear strength in X-Y plane.

Table 4.5 Material properties - Polypropylene/E-Glass [21]

Density 1850 kg/m3

E11, E22 14E9 Pa

E33 5.3E9 Pa

G12 1.8E9 Pa

G31, G32 0.75E9 Pa

21 0.08

31 0.14

32 0.15

XT 0.45E9 Pa

YT 0.45E9 Pa

ZT 0.15E9 Pa

37

YC 0.25E9 Pa

SC 0.032E9 Pa

Table 4.6 shows the material properties of the Projectile, Tool Steel.

Table 4.6: Material Properties of Tool Steel

Youngs Modulus, E 210E9 Pa

Poisson Ratio 0.28

Density 7870 kg/m3

Table 4.7 describes the geometry of a single ply of the composite laminate.

Table 4.7 Dimensions of Single ply

Length 50mm

Width 50 mm

Layer Thickness 0.68 mm

Table 4.8 denotes the dimensions of the projectile which is a cylinder

Table 4.8 Dimensions of Projectile

Radius 6.35 mm

Length 3.25 mm

4.5 Description of Cards

LS-DYNA is a highly developed Numerical code; it consists of vast library of

features. Every feature in LS-DYNA is described by a Card. Various material models are

designed to suit the different materials and fields of application.

38

In this research work mainly MAT_PLASTIC_KINEMATIC, MAT_RIGID,

MAT_COMPOSITE_DAMAGE are used.

4.5.1 MAT_PLASTIC_KINEMATIC

Material model MAT_PLASTIC_KINEMATIC was used to model the target. It has a

provision for element deletion with element failure strain when set to certain value. This

helps in removal of failed elements from calculation thus decreasing the computation time.

Isotropic hardening or kinematic hardening or combination of the both can be used by

varying a parameter from 0 to 1. In isotropic hardening, the center of the yield surface is

fixed but the radius is a function of the plastic strain. In kinematic hardening, the radius of the

yield surface is fixed but the center translates in the direction of the plastic strain.

4.5.2 MAT_RIGID

This material provides a convenient way of turning one or mode parts comprised of

beams, shells, or solid elements into rigid body. Approximating a deformable body as rigid is

a preferred modeling technique in many real world applications. Elements which are rigid are

bypassed in the element processing and no storage is allocated for storing history variables;

consequently, the rigid material is very cost efficient.

4.5.3 MAT_COMPOSITE_DAMAGE

The material model used for Composite should have orthotropic material properties

and also failure criteria. Chang-Chang Composite Failure Model developed by Chang is

damage model. MAT_COMPOSITE_DAMAGE model failed elements are not deleted from

computation. Since Lagrangian formulation is used severe distortions due to large

deformations of even one element will drastically reduce the time step size needed to find a

stable solution of the governing equations that will either stop computation or make them

extremely slow. This phenomenon is overcome by using MAT_ADD_EROSION, regarding

39

the material in the element to have failed when maximum principal strain is reached at its

centroid and deleting the failed element from the analysis.

4.5.4 INITIAL_VELOCITY_RIGID_BODY

Velocity for the bullet is given with INITIAL_VELOCITY_RIGID_BODY this card

gives velocity to all the nodes of the body and overrides any individual nodal velocities.

4.6 Modeling Contact

Contact treatment forms an integral part of many large-deformation problems.

Accurate modeling of contact interfaces between bodies is crucial to the prediction capability

of the finite element simulations. LS-DYNA offers a large number of contact types. Some

types are for specific applications, and others are suitable for more general use. Many of the

older contact types are rarely used but are still retained to enable older models to run as they

did in the past. Users are faced with numerous choices in modeling contact. This document is

designed to provide an overview of contact treatment in LS-DYNA and to serve as a guide

for choosing appropriate contact types and parameters.

4.7 How Contact Works

In LS-DYNA, a contact is defined by identifying (via parts, part sets, segment sets,

and/or node sets) what locations are to be checked for potential penetration of a slave node

through a master segment. A search for penetrations, using any of a number of different

algorithms, is made every time step. In the case of a penalty-based contact, when a

penetration is found a force proportional to the penetration depth is applied to resist, and

ultimately eliminate, the penetration. Unless otherwise stated, the contacts discussed here are

penalty-based contacts as opposed to constraint-based contacts. Rigid bodies may be included

in any penalty-based contact but in order that contact force is realistically distributed, it is

recommended that the mesh defining any rigid body be as fine as that of a deformable body.

40

Though sometimes it is convenient and effective to define a single contact that will handle

any potential contact situation in a model, it is permissible to define any number of contacts

in a single model. It is generally recommended that redundant contact, i.e., two or more

contacts producing forces due to the same penetration, be avoided by the user as this can lead

to numerical instabilities [23].

4.7.1 CONTACT_ERODING_SURFACE_TO_SURFACE

Erosion criterion in the contact provides additional advantage by deleting failed

elements from the calculation. It incorporates additional features like allocation of storage so

that erosion can occur, treatment of solid elements basing on boundary.

4.7.2 CONTROL_TIMESTEP

In explicit analysis LS-DYNA computes its own time step. Lagrangian formulation

users often come across messages of negative volume and abnormal termination. The time

strep scale factor in CONTROL_TIMESTEP has a default value of 0.9 which is not sufficient

for a stable calculation. So the TSSFAC value may be lowered to 0.67 for a stable

calculation.

4.7.3 CONTROL_CONTACT

This card allows controlling the sliding interface penalties in case of contacts. Small

interpenetration does happen always and obvious in case of high speed or impact loading.

So value of SLSFAC may be raised beyond 0.1. Besides this it allows controlling the friction,

contact thickness and offsets.

4.7.4 DATABASE_BINARY _D3PLOT

This card plots output data at predefined intervals of time. This helps in user to animate the

different stages of analysis by animation.

41

4.7.5 CONTROL_HOURGLASS

This option switches the hourglass formulation. By default LS-DYNA controls the hourglass

modes with available equal to 0.1. But for the present problem an hourglass coefficient of 6

and variable of 1 is very effective in preventing negative volumes and controlling the zero

energy modes.

42

CHAPTER 5

RESULTS AND DISCUSSIONS

5.1 Validation

The proposed model was analyzed in LS-DYNA for given loading and boundary

conditions. The outputs were studied in post processor LS-PREPOST and were compared

with results in literature and good correlation was found between the simulation and results of

Staley and Baker [1]. Table 5.1 shows three different cases of the impact. Residual velocity

of the impacted projectile is the only data provided in the experimental data. The simulation

results were in good agreement with the experimental values.

Table 5.1 Cases analyzed with FEA and compared with experimental results

Case Mass (kg)

Projectile Diameter

(m) L/D Plate Thick ness

(m)

1 0.001943 0.0075946 0.713 .003175

2 0.01555 0.0149098 0.767 0.0127

3 0.01555 0.0149098 0.767 0.00476

43

Table 5.1 (contd): Cases analyzed with FEA and compared with experimental results

Cases Incident velocity (m/s)

Experimental Residual Velocity

(m/s)

Simulation Residual velocity

(m/s)

Percentage Variation

1 1115.8728 545.896 540.40 1.017

2 1495.9587 630.936 700.5658 9.93

3 1791.3096 1739.4936 1830.9 4.992

5.2 Parametric study

A Parametric study was performed to understand the variation of the ballistic

response. Following cases in the tables were studied on validation case no. 1 of table 5.1.

table 5.2 describes the three cases with variation velocities and case 4 of Ballistic limit.

Ballistic limit was found by trial and error method. The remaining parameters like target

thickness, projectile mass, projectile geometry, failure strain are kept constant.

Table 5.2 Case: Velocity variation

Case no Velocity (m/s)

1 1200

2 1250

3 1300

4 Ballistic Limit

The table 5.3 describes the case of varying mass of the projectile for the model in case no. 1of

table 5.1. The mass of the projectile is scaled by scaling the density of the projectile. The

44

remaining parameters like target thickness, projectile mass, projectile geometry, projectile

velocity, failure strain are kept constant.

Table 5.3 Case: Projectile Mass variation

Case no Mass(kg)

1 0.00259

2 0.003239

3 0.003887

To understand the affect of geometry in impact on plate, shape of the projectile is changed to

spherical geometry for the validation case no.1 of the table 5.1.Two sphere diameters are

studied as shown in table 5.4. The remaining parameters like target thickness, failure strain

are kept constant.

Table 5.4 Case: Geometry variation (Sphere)

Case no Radius(m)

1 0.1495

2 0.2

For the model in validation case no.1, the projectile geometry is changed to sphere to a radius

0.2 in and velocity is varied as shown in three cases shown in table 5.5 keeping all the other

parameters as constant.

Table 5.5 Case: Spherical Projectile velocity

Case no Velocity(m/s)

1 1115.873

2 1200

3 1250

45

For the validation case no.1 table 5.1, failure strain of target material is varied to observe the

effect on the impact result keeping all other parameters constant.

Table 5.5 Case: Failure Strain Variation

Case no Failure strain

1 1.75

2 1.80

3 1.90

Three cases were studied for composite by varying the incident velocities as shown in the

table 5.6

Table 5.6 Case: Projectile Residual Velocity Variation in Composite Plate Impact

Case no Velocity (m/s)

1 125

2 187

3 200

Figurative description of all the above mentioned cases was shown in the next section.

Each case is expressed diagrammatically in four stages. Residual velocity of the projectile,

kinetic energy of the projectile and the internal energy rise in the target were plotted for each

of the cases.

Experimental work of this research doesnt have any data related to stress and strain

of the plate. No information was stated regarding the deformation of the projectile. So kinetic

energy of the projectile and internal energy rise in the plate are used to study the energy

distribution.

46

5.3 Validation case 1

Figure 5.1.1 Plate deformation

Figure 5.1.2 Residual Velocity of the Bullet

47

Figure 5.1.3 Kinetic Energy Lost by the bullet

Figure 5.1.4 Internal energy rise in the plate

48

From the figure 5.1.1 the sequence of stages of impact can be seen. Global bending or

dishing is observed in the third stage. The residual velocity curve depicted by the figure 5.1.2

shows linear variation up to 0.05 milliseconds and there by there was an influx up to 0.6

milliseconds. This may be due to the shearing action caused during plugging. Following the

Law of conservation of momentum, exchange of energies takes place between the projectile

and the plate. It can be observed from the figure 5.1.3 which shows kinetic energy lost by the

projectile and figure 5.1.4 which shows the internal energy gained by the plate.

5.3.2 Validation Case 2

Figure 5.2.1 Plate deformation

The figure 5.2.1 shows the sequence of stages of impact event. It can be observed that

the target does not undergo much deflection in normal direction. Instead of dishing little

spalling can be observed around the area of the impact.

49

Figure 5.2.2 Residual velocity of the projectile

Figure 5.2.3 KE lost by bullet

The figure 5.2.2 shows residual velocity of the projectile, the profile of the curve

appears different from the previous case. The influx was found to be less and curve goes

almost linear. The kinetic energy lost by the plate was depicted in the figure 5.2.3 and

internal energy gained by the projectile was given by figure 5.2.4.

50

Figure 5.2.4 IE rise in the Plate

5.3.3 Validation: Case 3

Figure 5.3.1 Plate deformation

51

Figure 5.3.2 Residual velocity of Bullet

Figure 5.3.3 KE lost by Bullet

Figure 5.3.4 IE rise in the Plate

52

The figure 5.3.1 shows the sequence of stages of impact of the plate. In comparison

with two previous cases the dishing was found to be comparatively less. Spalling was to be

more compared to other case this can be because of higher thickness of the target. The

amount of energy lost to the eroded mass increases with the thickness.

5.4 BALLISTIC LIMIT

Figure 5.4.1 Plate deformation

Figure 5.4.1 above shows the plate in validation case no.1 of table 5.1 at the ballistic limit. It

clearly explained the behavior of the plate at the ballistic limit. The phenomena of dishing

took place which could be seen in the last stage of the sequence. The dishing or stretching

was at its maximum in the case of ballistic limit.

53

Figure 5.4.2: Residual velocity

Figure 5.4.3 KE lost by projectile

Figure 5.4.2 shows the velocity degradation as the projectile was completely stopped

by the target .Figure 5.4.3 shows kinetic energy of the projectile was completely lost by the

projectile in duration of 3 milliseconds. Following the Law of Conservation the kinetic

energy lost by the projectile was gained by the target as shown by internal energy rise in the

figure 5.4.4. Some portion of energy may be lost to friction and heat generation.

54

Figure 5.4.4 IE gained by plate

5.5.1 Case: Projectile Mass: 0.00259kg

Figure 5.5.1 Plate deformation

55

Figure 5.5.2 Residual velocity of Bullet

Figure 5.5.3 KE lost by Bullet

Figure 5.5.1 shows the impact sequence when projectile in the validation case 1 of

table 5.1 was increased to 0.00259 kg. The figure 5.5.2 shows the velocity degradation with

respect to time. The residual velocity increased compared to the validation case 1. The

projectile reaches stable velocity soon after 0.5 milliseconds.

56

Figure 5.5.4 IE rise in the Plate

5.5.2 Case: Projectile mass: 0.003239 kg

Figure 5.6.1 Plate deformation The figure 5.6.1 shows the stages impact event with mass of projectile increased to

0.003239kg in the validation case 2.

57

Figure 5.6.2 Residual velocity of projectile

Figure 5.6.3 KE lost by projectile

Figure 5.6.2 shows the velocity degradation of the projectile with respect time

residual velocity increased to 821 m/s. Figure 5.6.3 shows the amount of kinetic energy lost

58

by the projectile. The amount of internal energy gained by the plate was shown by the figure

5.6.4.

Figure 5.6.4 IE rise in the Plate

5.5.3 Case: Projectile Mass: 0.003887kg

Figure 5.7.1 Plate deformation

59

Figure 5.7.1 shows the stages of impact projectile of mass increased to 0.003887kg in the

validation case 1 of table 5.1

Figure 5.7.2 Residual velocity of Bullet

Figure 5.7.3 KE lost by Bullet

From the figure 5.7.2 the residual velocity of the projectile increased to 882m/s with

increase in projectile mass. The kinetic energy lost by the bullet and the internal rise in the

target are shown in the figure 5.7.3 and figure 5.7.4 respectively. The amount of internal

60

energy rise in the target doesnt appear to increase much. This shows that there was constant

energy absorption by the eroded mass.

Figure 5.7.4 IE rise in the Plate

Projectile Mass Variation

720

740

760

780

800

820

840

860

880

900

0 0.001 0.002 0.003 0.004 0.005

Mass of Projectile (kg)

Vel

ocity

of P

roje

ctile

(m/s)

Figure 5.7.5 Residual velocity variation with variation in projectile mass

61

The three cases of the varying mass of the projectile as tabulated in table 5.2 can be

summarized as shown in the figure 5.7.5. Increase in residual velocity with increase in mass

of the projectile increases.

5.6.1 Case: Projectile Velocity: 1200 m/s

Figure 5.8.1 Plate deformation Figure 5.8.1 shows the sequence of stages of projectile impact for velocity of the projectile

increased to 1200m/s. The figure 5.8.1 shows the increased residual velocity of the projectile.

The kinetic energy lost by projectile and internal gained by the projectile were shown by the

figures 5.8.3 and 5.8.4.

62

Figure 5.8.2 Residual velocity of Bullet

Figure 5.8.3 KE lost by bullet

63

Figure 5.8.4 IE rise in the Plate

5.6.2 Case: Projectile Velocity: 1250m/s

Figure 5.9.1 Plate deformation Figure 5.9.1 shows the stages of the projectile with incident velocity increased to

1250 m/s. The kinetic energy lost by the projectile and Internal energy gained by the Plate

64

were shown by the figures 5.9.3 and 5.9.4. The internal energy rise in the target was almost

same as the kinetic energy gained by the target.

Figure 5.9.2 Residual velocity of Bullet

Figure 5.9.3 KE lost by Bullet

65

Figure 5.9.4 IE rise in the Plate

The internal energy rise in the target was less compared to previous velocity case.

5.6.3 Case: Projectile Velocity: 1300m/s

Figure 5.10.1 Plate deformation

The figure 5.10.1 shows the four stages in impact of projectile with incident velocity 1300

m/s. The residual velocity graph with respect to time was shown in figure 5.10.2.

66

Figure 5.10.2 Residual velocity of Bullet

Figure 5.10.3 KE lost by Bullet

The figure 5.10.3 and 5.10.4 show the kinetic energy lost by the bullet and the internal gained

by the projectile. The internal rise in the target was lesser than the two of previous cases of

velocity.

67

Figure 5.10.4 IE rise in the Plate

Incident Veloci